1 / 58

# Effect of Symmetry on the Orientation Distribution - PowerPoint PPT Presentation

Effect of Symmetry on the Orientation Distribution. 27-750, Fall 2009 Texture, Microstructure & Anisotropy, Fall 2009 A.D. Rollett, P. Kalu. Last revised: 22 nd Apr. ‘11. Objectives.

I am the owner, or an agent authorized to act on behalf of the owner, of the copyrighted work described.

## PowerPoint Slideshow about 'Effect of Symmetry on the Orientation Distribution ' - galia

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -
Presentation Transcript

### Effect of Symmetry on the Orientation Distribution

27-750, Fall 2009

Texture, Microstructure & Anisotropy, Fall 2009

A.D. Rollett, P. Kalu

Last revised: 22nd Apr. ‘11

• Review of symmetry operators, their matrix representation, and how to use them to find all the symmetrically equivalent descriptions of a given texture component.

• To illustrate the effect of crystal and sample symmetry on the Euler space required for unique representation of orientations.

• To explain why Euler space is generally represented with each angle in the range 0-90°, instead of the most general case of 0-360° for 1 and 2, and 0-180° for .

• To point out the special circumstance of cubic crystal symmetry, combined with orthorhombic sample symmetry, and the presence of 3 equivalent points in the 90x90x90° “box” or “reduced space”.

• To explain the concept of “fundamental zone”.

• Part 1 of the lecture provides a qualitative description of symmetry and its effects. Part 2 provides the quantitative description of how to express symmetry operations as rotation matrices and apply them to orientations.

Crystal vs. Sample Symmetry

• An understanding of the role of symmetry is essential in texture.

• Two separate and distinct forms of symmetry are relevant:

• CRYSTAL symmetry

• SAMPLE symmetry

• Crystal symmetry is always present (even if, in principle, heavily defected crystals may exhibit lower symmetry) and must always be accounted for. Sample symmetryis only present on a statistical basis, i.e. only a polycrystal can exhibit sample symmetry for the texture as a whole.

• Typical usage lists the combination crystal-sample symmetry in that order, e.g. cubic-orthorhombic.

Concept Params. Euler Normalize Vol.Frac. Cartesian Polar Components

The essential points of this lecture are:

• Crystal symmetry means that a crystal can be rotated in various ways that leave it unchanged (physically indistinguishable). In orientation space, the equivalent result is that any given orientation is related to exactly as many other orientations as there are symmetry operators (understandable in terms of group theory).

• Because there are multiple equivalent points, we usually divide up the full orientation space (e.g. 360°x180°x360° in Euler space) and use only a small portion of it (e.g. 90°x90°x90°).

• Sample symmetry has the same sort of effect as crystal symmetry, even though it is a statistical symmetry (and orientations related by a sample symmetry element are physically distinguishable and do have a misorientation between them. Sample symmetry is evident in pole figures whereas crystal symmetry is evident in inverse pole figures.

• Unfortunately, Euler space (spherical angles) means that the dividing planes have odd shapes and so for the common cubic-orthorhombic combination, we have 3 copies of the fundamental zone in the range 0-90° for each angle. Rodrigues space is far simpler in this respect because symmetry operators always lead to flat dividing planes.

Deformation vs. Sample Symmetry

• Note that the texture of a material is a product of its history.

• The (statistical) sample symmetry is directly related to the symmetry of the preceding deformation.

• In general, the sample symmetry reflects the lowest symmetry deformation.

• Rolling is a plane strain deformation, with orthorhombic symmetry. Torsion is a simple shear, with monoclinic symmetry. Wire drawing is an axi-symmetric deformation with cylindrical symmetry.

{111}

• (111) pole figure showing a maximum intensity at a specific angle from a particular direction in the sample, and showing an infinite rotational symmetry (C).

• F.A.=Fiber Axis

• A particular crystal direction in all crystals is aligned with this fiber axis.

• For a cubic material, this combination would be classed as cubic-cylindrical.

In this case, <100> // F.A.

• Illustration of 3-fold, 4-fold, 6-fold rotational symmetry

The essential point about applying a symmetry operation is that, once it has been done, you cannot tell that anything has changed. In other words, the rotated or reflected object is physically indistinguishable from what you started with.

Note the symbols used to denote the different rotational symmetry elements.

• Note how one can re-label the axes but leave the physical object (crystal) unchanged.

• Which symmetry operator was applied (from O(432))?

[001]

[100]

[010]

[010]

[001]

[100]

Stereographic projectionsof symmetry elements and general poles in thecubic point groupswith Hermann-Mauguinand Schoenflies designations.

Note the presence of four triad symmetry elements in all these groups on <111>.

Cubic metals mostlyfall under m-3m.

Groups: mathematical concept, very useful for symmetry

Torsion, shear:Monoclinic, 2.

Rolling, plane straincompression, mmm.

Otherwise,triclinic.

Axisymmetric: C

• The fundamental zone (or asymmetric unit) is the portion or subset of orientation space within which each orientation (or misorientation, when we later discuss grain boundaries) is described by a single, unique point.

• The fundamental zone is the minimum amount of orientation space required to describe all orientations.

• Example: the standard stereographic triangle (SST) for directions in cubic crystals.

• The size of the fundamental zone depends on the amount of symmetry present in both crystal and sample space. More symmetry  smaller fundamental zone.

• Note that in Euler space, the 90x90x90° region typically used for cubic [crystal]+orthorhombic [sample] symmetry is not a fundamental zone because it contains 3 copies of the actual zone!

• Crystal symmetry operates in a frame attached to the crystal axes.

• Based on the definition of Euler angles, crystal symmetry elements produce relations between the second & third angles.

• Sample symmetry operates in a frame attached to the sample axes.

• Sample symmetry produces relations between the first & second angles.

• The combination of crystal and sample symmetry is written as crystal-sample, e.g. cubic-orthorhombic, or hexagonal-triclinic.

• Four-fold rotation elements (and mirrors in the orthorhombic group) are used to limit the third, f2, (first, f1) angle range to 0-90°.

• Second angle, F, has range 0-90° (diffraction adds a center of symmetry).

Section SizesCrystal - Sample

• Cubic-Orthorhombic: 0f1 90°, 0F90°, 0f2 90°

• Cubic-Monoclinic: 0f1 180°, 0F90°, 0f2 90°

• Cubic-Triclinic: 0f1 360°, 0F90°, 0f2 90°

• But, these limits do not delineate a fundamental zone.

f2

Points related by triad symmetryelement on <111>(triclinicsample symmetry)

F

f1

Take a point, e.g. “B”; operate on it with the 3-fold rotation axis (blue triad); the set of points related by the triad are B, B’, B’’, with B’’’ being the same point as B. The point is, that as you operate on a point (orientation) with a symmetry operation, in general all the Euler angles change.

[Bunge]

The “S” component,{123}<634>

has angles {59, 37, 63}also {27,58,18},{53,74,34}

and occurs in three

related locations

in Euler space. 10° scattershown about component.

Regions I, II and III are

symmetry element,

Randle & Engler, fig. 5.7

section

in f1 cuts

through

more than

one subspace

[Bunge]

S component in f2 sections

Regions I, II and III are

symmetry element,

Randle & Engler, fig. 5.7

• O(432) has 24 operators (i.e. order=24); O(222) has 4 operators (i.e. order=4): why not divide the volume of Euler space (8π2, or, 360°x180°x360°) by 24x4=96 to get π2/12 (or, 90°x30°x90°)?

• Answer: we leave out a triad axis (because of the awkward shapes that it would give us), so we divide by 8x4=32 to get π2/4 (90°x90°x90°).

• This is an illustration of group theory in action. Each set of symmetry operators divides up the orientation space by a factor equal to the number of elements in the group.

• The reason is, essentially, a question of counting: each point in one zone has exactly one point in another zone related by a given operator.

f1=0°

360°

180°

270°

90°

F

‘mirror’

‘mirror’

= 180°

2-fold screw axis changes f2by π

Note: this slide illustrates how the set of 3 diads (+ identity) in sample space operate on a given point. The relationship labeled as ‘mirror’ is really a diad that acts like a 2-fold screw axis in Euler space.

Tables for Texture Analysis of Cubic Crystals, Springer Verlag, 1978

3-fold axis

360°

180°

270°

90°

f2=0°

F

4-fold axis

Other 4-fold, 2-fold axis:act on f1 also

= 180°

Note: points related by triad (3-fold) have different f1 values.

Tables for Texture Analysis of Cubic Crystals, Springer Verlag, 1978

• For cubic-orthorhombic crystal+sample symmetry, we use a range 90°x90°x90° for the three angles, giving a volume of 90°2 (or π2/4 in radians).

• In the (reduced) space there are 3 equivalent points for each orientation (texture component). Both sample and crystal symmetries must be combined together to find these sets.

• Fewer (e.g. Copper) or more (e.g. cube) equivalent points for each component are found if the the component coincides with one of the symmetry elements.

• Again, this is an illustration of group theory in action. Each set of symmetry operators divides up the orientation space by a factor equal to the number of elements in the group.

• Crystal symmetry:a combination of 4- and 2-fold crystal axes (2x4=8 elements) reduce the range of Ffrom π to π/2, and f2 from 2π to π/2.

• Sample symmetry:the 2-fold sample axes (4 elements in the group) reduce the range of f1 from 2π to π/2.

• Volume of {0  f1, F, f2  π/2} is π2/4.

• The reason is, essentially, a question of counting: each point in one zone has exactly one point in another zone related by a given operator.

No. of points in the 90x90x90° space

Copper:2

Brass:3

S:3

Goss:3

Cube:8

Dillamore: 2

Why this variation?Points that fall on the edge may appear more, or fewer times than the standard count of 3.

Humphreys & Hatherly

f1=0°

360°

180°

270°

90°

F

= 90°

Cube lies on the corners

Copper, Brass, Goss lie on an edge, so that they coincide with a symmetry element

3D Views Space

a) Brass b) Copper c) S d) Goss e) Cube f) combined texture

1: {35, 45, 90}, Brass,

2: {55, 90, 45}, Brass

3: {90, 35, 45}, Copper,

4: {39, 66, 27}, Copper

5: {59, 37, 63}, S,

6: {27, 58, 18}, S,

7: {53, 75, 34}, S

8: {90, 90, 45}, Goss 9: {0, 0, 0}, cube* 10: {45, 0, 0}, rotated cube

* Note that the cube exists as a line between (0,0,90) and (90,0,0) because of the linear dependence of the 1st and 3rd angles when the 2nd angle = 0.

Figure courtesy of Jae-hyung Cho

• Points coincident with symmetry axes may also have equivalent points, often on the edge. Cube: should be a single point, but each corner is equivalent and visible.

• Goss, Brass: a single point becomes 3 because it is on the f2=0 plane.

• Copper: 2 points because one point remains in the interior but another occurs on a face; also the Dillamore orientation.

• Note for later about volume fractions: although the volumes enclosed by the 12° capture (misorientation) distance shown in the figure vary with the 2nd euler angle, to first order it is the symmetry planes that control the volume fractions. So S, for example, has 3 complete “blobs” whereas Goss has only 3 x ¼ and so will contain only ~1/4 of the volume fraction of S, based on a random (uniform) texture.

Part 2: Quantitative Space

• In part 2 of the lecture, we describe the methods for describing symmetry operations as rotation matrices and how to apply them to texture components, also expressed as matrices.

• Notation:orientation: g(crystal) symmetry operator: OC(sample) symmetry operator: OS

• Rotational symmetry elements exist whenever you can rotate a physical object and result is indistinguishable from what you started out with.

• Rotations can be expressed in a simple mathematical form as unimodular matrices, often with elements that are either one or zero (but not always!).

• When represented as matrices, the inverse of a rotation is equal to the transpose of the matrix.

• Rotations are transformations of the first kind; determinant = +1.

• Reflections (not needed here) are transformations of the second kind; determinant = -1.

• Crystal symmetry also can involve translations but these are not included in this treatment.

• Multiply each set of three coefficients taken along a diagonal: top left to bottom right are positive, bottom left to top right negative.

• |a| = a11a22a33+a12a23a31+a13a21a32- a13a22a31-a12a21a33-a11a32a23=ei1i2…inai11ai22…aiNN

-

+

• Since crystal symmetry operators are closely linked to low index directions, it is helpful to convert axis-angle descriptions to matrices and vice versa.

• The rotation can be converted to a matrix, g, (passive rotation) by the following expression, whered is the Kronecker delta,  is the rotation angle, r is the rotation axis, and e is the permutation tensor.

Compare with active rotation matrix!

Written out as a complete 3x3 matrix:

• Diad on z: [uvw] = [001],  = 180° - substitute the values of uvw and angle into the formula

• 4-fold on x: [uvw] = [100] = 90°

- Space

Matrixrepresentation of the rotation point groups

What is a group? A group is a set of objects that form a closed set: if you combine any two of them together, the result is simply a different member of that same group of objects. Rotations in a given point group form closed sets - try it for yourself!

Note:the 3rd matrix in the 1st column (x-diad) is missing a “-” on the 33 element; this is corrected in this slide. Also, in the 2nd from the bottom, last column: the 33 element should be +1, not -1. In some versions of the book, in the last matrix (bottom right corner) the 33 element is incorrectly given as -1; here the +1 is correct.

Kocks: Ch. 1 Table II

• In general, the notation identifies the axis about which the rotation is performed.

• Thus a 2-fold axis (180° rotation) about the z-axis is known as a z-diad, or C2z, or L0012

• A group is written as O(432), for example, where the entry in the parentheses indicates the symmetry.

• Convert Miller indices that represent an orientation or texture component to a (orientation) matrix.

• Perform matrix multiplication with the symmetry operator, Oc, and the orientation matrix, g, to obtain the new orientation (matrix), g’. Be careful to get the order correct! For the standard coordinate/axis transformation used here, the crystal symmetry operator always left-multiplies (pre-multiplies) the orientation. Since the orientation matrix converts from sample to crystal axes, you can think of applying crystal symmetry after transforming a quantity into the crystal frame.

• g’ = OC g

• Convert the matrix back to Miller indices.

• The two sets of indices represent (for crystal symmetry) indistinguishable objects.

Example Space

g’ = OC g

g

Goss: {110}<001>:

=

OC

g

which is {-1-10}<001>

g’

Sample symmetry: right multiply (post-multiply) the matrix.

Crystal symmetry SpaceO(432) acting on the (231)[3-46] S component

Note that all 24 variants are present

Homework exercise: you can make this same plot by using, e.g., Excel to compute the matrix of each symmetrically equivalent orientation and then converting the matrix to Euler angles.

Order of Matrices Space

• Assume that we are using the standard axis transformation (passive rotation) definition of orientation (as found, e.g. in Bunge’s book).

• Order depends on whether crystal or sample symmetry elements are applied.

• For an operator in the crystal system, Oxtal, the operator pre-multiplies the orientation matrix.

• Think of the sequence as first transform into crystal coordinates, then apply crystal symmetry once you are in crystal coordinates.

• For sample operator, Osample, post-multiply the orientation matrix.

• Note that the result of applying any available operator is equivalent to (physically indistinguishable in the case of crystal symmetry) from the starting configuration (not mathematically equal to!).

• Also, if you apply a sample symmetry operator, the result is generally physically different from the starting position. Why?! Because the sample symmetry is only a statistical symmetry, not an exact, physical symmetry.

• Do not confuse this with the standard expression for the transformation of a second rank tensor: T’ = OTOT

NB: if one writes an orientation as an active rotation (as in continuum mechanics), then the order of application of symmetry operators is reversed: premultiply by sample, and postmultiply by crystal!

• For later: when you use a material property (of a single crystal, for example) to connect two physical quantities, then applying symmetry means that the result is unchanged. In this case there is an equality. This equality allows us to decrease the number of independent coefficients required to describe an anisotropic property (Nye).

Anisotropy Space

• Given an orientation distribution, f(g), one can write the following for any tensor property or quantity, t, where the range of integration is over the fundamental zone of physically distinguishable orientations, SO(3)/G.

• “SO(3)” means all possible proper rotations in 3D space (but not reflections); “G” means the set (group) of symmetry operators, e.g. (432) for the proper rotations in the cubic system; SO(3)/G means the space of rotations divided by the symmetry group.

• Each symmetry operator relates a pair of points in orientation (Euler) space.

• Therefore each operator divides the available space by a factor of the order of the rotation axis. In fact, the order of group is significant. If there are four symmetry operators in the group, then the size of orientation space is decreased by four.

• This suggests that the orientation space is smaller than the general space by a factor equal to the number of general poles.

Symmetry: How-to Space

• How to find all the symmetrically equivalent points?

• Convert the component of interest to matrix notation.

• Make a list of all the symmetry operators in matrix form (24 for cubic crystal symmetry or 12 for hexagonal crystal symmetry, and 4 for orthorhombic sample symmetry). This is the same list of operators shown as 3x3 matrices in the Table quoted from the Kocks book, slide 35 in this set.

• Crystal symmetry: identity (1), plus 90/180/270° about <100> (9), plus 180° about <110> (6), plus 120/240° about <111> (8).

• Sample symmetry: identity, plus 180° about RD/TD/ND (4).

• Loop through each symmetry operator in turn, with separate loops for sample and crystal symmetry.

• For each result, convert the matrix to Euler angles.

Homework Space

• This describes the part of the homework (Hwk 3) that deals with learning how to apply symmetry operators to components and find all the symmetrically related positions in Euler space.

• A. Write the symmetry operators for the cubic crystal symmetry (point group 432) as matrices into a file. It is sensible to put three numbers on a line, so that the appearance of the numbers is similar to the way in which a 3x3 matrix is written in a book. You can simply copy what was given in the slides (taken from the Kocks book).

• [Alternatively, you can work out what each matrix is based on the actual symmetry operator. This is more work but will show you more of what is behind them.]

• B. Write the symmetry operators for the orthorhombic sample symmetry (point group 222) as matrices into a separate file.

• C. Write a computer code that reads in the two sets of symmetry operators (cubic crystal, asks for an orientation specified as (six) Miller indices, (h,k,l)[u,v,w], and calculates each new orientation, which should be written out as Euler angles (meaning, convert the result, which is a matrix, back to Euler angles). Note that the identity operator is always include as the first symmetry operator. So, even if you apply no symmetry, in terms of loops in your program, you go at least once through each loop where the first time through is applying the identity operator (ones on the diagonal, zeros elsewhere).

• D. List all the equivalent points for {123}<63-4> for triclinic (meaning, no sample symmetry). In each listing, identify the points that fall into the 90x90x90 region typically used for plotting.

• E. List all the equivalent points for {123}<63-4> for monoclinic (use only the ND-diad operator, i.e. 180° about the sample z-axis). In each listing, identify the points that fall into the 90x90x90 region typically used for plotting.

• F. List all the equivalent points for {123}<63-4> for orthorhombic sample symmetries (use all 3 diads in addition to the identity). In each listing, identify the points that fall into the 90x90x90 region typically used for plotting.

• G. Repeat 3f above for the Copper component, (112)[11-1].

• H. How many different points do you find for each of the three sample symmetries?

• I. How many points fall within the 90x90x90 region that we typically use for plotting orientation distributions?

• Students may code the problem in any convenient language (Excel, C++, Pascal….): be very careful of the order in which you apply the symmetry operators!

• How can you be sure that you have applied the operators correctly? Answer: make a pole figure of the set of symmetrically related orientations. Crystal symmetry related points must plot on top of one another whereas sample symmetry related points give rise to (in general) multiple sets of points, related by the sample symmetry that should be evident in the pole figure.

Discussion Points Space

• If we change the sample symmetry to monoclinic, how large a space should we use in Euler angle space?

• If we change the crystal symmetry to hexagonal, how does this change the range of Euler angles required? Can you explain why the 3rd Euler angle only needs to have the range 0-60°?

Summary Space

• Symmetry operators have been explained in terms of rotation matrices, with examples of how to construct them from the axis-angle descriptions.

• The effect of symmetry on the range of Euler angles needed, and the shape of the plotting region.

• The particular effect of symmetry on certain named texture components found in rolled fcc metals has been described.

• In later lectures, we will see how to perform the same operations but with or on Rodrigues vectors and quaternions.

Supplemental Slides Space

• The following slides provide:

• Details of the range of Euler angles, and the shape of the plotting space required for CODs (crystallite orientation distributions) or SODs (sample orientation distributions) as a function of the crystal symmetry;

• Additional information about the details of how symmetry elements relate different locations in Euler space.

Sample Symmetry Element Spacee.g. diad on ND(associated with f1)

Crystal Symmetry Elemente.g. rotation on [001](associated with f2)

[Bunge]

[Kocks] Space

These are simple cases: see detailed charts at the end of this set of slides

• Symmetry operators of the second kind: these operators include the inversion center and mirrors; determinant = -1.

• The inversion (= center of symmetry) simply reverses any vector so that (x,y,z)->(-x,-y,-z).

• Mirrors operate through a mirror axis. Thus an x-mirror is a mirror in the plane x=0 and has the effect (x,y,z)->(-x,y,z).